. The data used in scaling analysis has been corrected for demagnetization factor.

The x-ray data has been analyzed by the Rietveld refinement method using FULLPROF software[@Carvajal] and the results show that the sample is single phase and crystallizes in rhombohedral structure with space group R-3c which is in agrement with the previous report.[@Fita] Figure \[fig: XRD\] displays the room temperature x-ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ along with its Rietveld fit profile. The goodness of fitting $\chi^2$ is 1.26 and the lattice parameters of the unit cell are a=5.4549(2) and c=13.3194(2). The oxygen content is determined by thermogravimetric analysis which is close to its stoichiometric value of 3.0.

![(Color online) X-ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ at room temperature. The solid circles represents the experimental X-ray diffraction data, the red line on the experimental data exhibits the Rietveld refinement for rhombohedral R-3c structure with $\chi^2$=1.26, the short vertical lines show the Bragg peak positions, and the bottom blue line displays the difference between the experimental and calculated pattern.[]{data-label="fig: XRD"}](Fig1.eps){width="0.6\columnwidth"}

Results and Discussions
=======================

Thermomagnetic irreversibility
------------------------------

Figure \[fig: MT\] shows the magnetization versus temperature curves at the field of 5 Oe, 100 Oe, 500 Oe, and 10000 Oe in field cooled (FC) and zero field cooled (ZFC) protocols. In FC protocol the sample is cooled to 5 K in presence of applied field and data is recorded in heating run without changing the field. In ZFC protocol the sample is cooled to 5 K in zero field, then field is applied, and data is recorded in the heating run. Both FC and ZFC magnetization curves exhibit a paramagnetic to ferromagnetic transition on cooling and the transition temperature (T$_C$) is estimated to be around 203 K by the temperature derivative of the 500 Oe FC magnetization curve (see inset of Fig. \[fig: MT
. The data used in scaling analysis has been chastise for demagnetization agent. 

 The x - ray data has been analyze by the Rietveld refinement method use FULLPROF software[@Carvajal ] and the resultant role show that the sample distribution is individual phase and crystallizes in rhombohedral social organization with space group R-3c which is in agrement with the previous report.[@Fita ] Figure   \[fig: XRD\ ] displays the room temperature ten - ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3 $ along with its Rietveld fit profile. The goodness of match $ \chi^2 $ is 1.26 and the lattice parameters of the unit cellular telephone are a=5.4549(2) and c=13.3194(2). The oxygen content is determined by thermohydrometric analysis which is airless to its stoichiometric value of 3.0. 

! [ (Color online) X - beam diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3 $ at room temperature. The solid circles typify the experimental X - ray diffraction data, the red line on the experimental datum exhibit the Rietveld refinement for rhombohedral R-3c structure with $ \chi^2$=1.26, the short vertical lines show the Bragg peak positions, and the bottom blue channel displays the difference between the experimental and deliberate pattern.[]{data - label="fig: XRD"}](Fig1.eps){width="0.6\columnwidth " } 

 result and discussion 
 = = = = = = = = = = = = = = = = = = = = = = = 

 Thermomagnetic irreversibility 
 ------------------------------ 

 Figure   \[fig: MT\ ] shows the magnetization versus temperature curve at the battlefield of 5   Oe, 100   Oe, 500   Oe, and 10000   Oe in field cooled (FC) and zero airfield cooled (ZFC) protocols. In FC protocol the sample is cooled to 5   K in bearing of applied field and data is recorded in heating run without changing the plain. In ZFC protocol the sample is cooled to 5   K in zero field, then field is practice, and data is recorded in the heating streak. Both FC and ZFC magnetization curves exhibit a paramagnetic to ferromagnetic transition on cooling and the conversion temperature (T$_C$) is estimated to be around 203   thousand by the temperature derivative of the 500   Oe FC magnetization curvature (see insert of Fig.   \[fig: MT
. Thf data used in scaling akalysis has been correcved for demagnegization factor.

The x-ray data hqs betu analyzed by the Ridtveld revinement metiod using FULLPROF software[@Carbwjal] end the results show that the sample is sknyle phase and crystallizes in rhomboredral xtgucture with skace bwoup G-3c which is in agrement with ths previmus report.[@Fits] Figure \[fig: XRD\] displays tje rlom temperature x-rwy diffractuon [qttern of La$_{0.75}$Ca$_{0.25}$CoO$_3$ along with its Rjetveld fit profile. The goodnesr of yitting $\chi^2$ iw 1.26 wtd the lattmce pagameters of tmv unit well arr a=5.4549(2) and c=13.3194(2). The pxyjen xontent is determined by thermogravimettic analyshs which is close ti uts sjoichhomegeic vamux or 3.0.

![(Colog oiline) X-ray siffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ ae room temperafure. Tre solid circles represents the experimenual X-day diffraction data, thw red line on the expgrimental qata exhibits the Rietveld refinement for rhombohadral F-3c wtvuctjee with $\chi^2$=1.26, the short vertical lines show the Bwzgb ieak positions, anb the bottom blur pimg displays the diffexsnde between the expfrimentwl ane calculaued psttern.[]{data-label="fig: XRD"}](Fig1.epw){width="0.6\columncidrh"}

Results and Discbssions
=======================

Thermumagmetic irreversibility
------------------------------

Figure \[fng: MT\] ahows the mwgnetizatjun versus temperxtuge cgrves at the field of 5 Oe, 100 Oq, 500 Oe, and 10000 Ie iu field zoolgd (FC) agd zero fifld cooled (ZFC) protocols. In FE prodocol the dample is cooled to 5 K in presenrx of applied giald and datc is rccorded in heatyng run withouj changiny the wield. In ZRC protmcol the saiple is cooleg to 5 K in zerm field, ehen fieod is aoolied, and data is recorbtd in the yeating run. Both FG and AFC magnetizatiin xurves exhibit s pxraiahnxtic em ferromagnedic gravxitiov on coolinn avd tne transition temperdturs (T$_C$) is estimated yo be aroubd 203 K by ehe temperatute derivative of tje 500 Oe FC magnrtieation curve (see inset of Fig. \[fif: MT
. The data used in scaling analysis corrected demagnetization factor. x-ray data has refinement using FULLPROF software[@Carvajal] the results show the sample is single phase and in rhombohedral structure with space group R-3c which is in agrement with the report.[@Fita] Figure \[fig: XRD\] displays the room temperature x-ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ with Rietveld profile. goodness of fitting $\chi^2$ is 1.26 and the lattice parameters of the unit cell are a=5.4549(2) c=13.3194(2). The oxygen content is determined by thermogravimetric which is close to stoichiometric value of 3.0. ![(Color X-ray pattern of at temperature. solid circles represents experimental X-ray diffraction data, the red line on the experimental data exhibits the Rietveld refinement for rhombohedral structure with short vertical show Bragg positions, and the line displays the difference between the pattern.[]{data-label="fig: XRD"}](Fig1.eps){width="0.6\columnwidth"} Results and Discussions ======================= Thermomagnetic irreversibility Figure \[fig: shows the magnetization versus temperature curves the field of 5 Oe, 100 Oe, 500 and 10000 Oe in field cooled (FC) and zero field cooled (ZFC) protocols. In FC sample is cooled to K in presence applied and is in heating without changing the field. In ZFC protocol the sample is cooled 5 K in zero field, then field is applied, and recorded the heating run. FC and ZFC magnetization exhibit paramagnetic to ferromagnetic transition and transition estimated be 203 K by the derivative of the 500 Oe magnetization curve (see inset
. The data used in scaling analySis has been CorreCteD foR dEmagNetiZation factor.

ThE X-ray Data has been analyzed by tHe RieTvELd reFInEment Method uSInG fuLLpRoF SofTwARe[@carvaJal] And the rEsults show ThaT tHe sample is siNGlE phase and cRysTallizes in rhOmbOhedraL sTruCTure wIth Space Group R-3C Which iS in agremeNt WIth the PRevious REPoRt.[@FiTa] Figure \[fig: XRD\] disPLaYS the room temperAture x-RaY DiFFRacTioN pattern of la$_{0.75}$ba$_{0.25}$CoO$_3$ ALong witH ItS rIEtvELd fit profile. THe goodness oF FitTing $\chI^2$ iS 1.26 anD The latTice pArAMetErs of the uniT celL are a=5.4549(2) and c=13.3194(2). the oxyGEn conteNT is deteRmined By tHerMogrAViMeTriC aNAlySIs WhiCH is Close to iTs StOichiOmetRIC VAlue Of 3.0.

![(COlor OnlinE) X-ray diffractIon PattERn oF La$_{0.75}$Ba$_{0.25}$coO$_3$ at Room TeMperaTure. ThE soliD cIrcles representS the ExperimenTal x-rAy dIfFractIOn data, The Red Line on tHe experIMenTaL DATa Exhibits the RietvelD rEFInEment for RhomboHEdRaL r-3c structUrE wiTh $\chI^2$=1.26, THe shoRt veRTiCal lines Show thE brAgG peak poSiTions, aNd The BotTom blUE linE displAys the diFfereNCe between the exPErimental and cALcULAtED patTerN.[]{data-label="fIg: XRd"}](fig1.ePs){wiDTh="0.6\ColUMnwidTh"}

ResUlTS aND Discussions
=======================

ThermomAgNetic iRreveRsibility
------------------------------

FiguRe \[fig: MT\] shoWS THe magnetIzatIOn VErsus temperatuRe curVes at the fiELd of 5 Oe, 100 Oe, 500 oe, and 10000 oe in fielD cooled (FC) AND zero fieLd cOolEd (ZfC) pROToCols. In FC protoCOL the SaMple is cOolEd to 5 K in PreSenCe oF apPlIed field aNd data is ReCoRdEd In hEatinG Run withoUt ChaNgIng The fiELd. In ZFc protOcol ThE sAMplE is coolED tO 5 k In zeRo FiEld, tHen FiEld is ApplIEd, aNd data iS recorded In tHE heaTiNg Run. Both fC and ZFC magneTiZation curvEs ExhIbit a pARAmagnetiC to ferromagnetic transitIOn on cooLinG and tHe trAnsition tEmpEraturE (T$_C$) IS estimAted to Be aroUnD 203 K bY THe temPERaTurE dErivative oF THe 500 OE FC maGnEtizAtion cuRve (see inset of Fig. \[fiG: mT
. The data used in scaling  analysishas b een  co rr ecte d fo r demagnetizat i on f actor.

The x-ray data  hasbe e n an a ly zed b y the R i et v e ldre fi nem en t  m ethod  us ing FUL LPROF soft war e[ @Carvajal] a n dthe result s s how that the  sa mple i ssin g le ph ase  andcrysta l lizesin rhombo he d ral st r ucturew i th  spa ce group R-3c whi c hi s in agrementwith t he pr e v iou s r eport.[@Fi ta ] Fig u re \[fi g :X R D \]d isplays the r oom tempera t ure  x-ray  d iff r action  patt er n  of  La$_{0.75} $Ba$ _{0.25}$C oO$_3$ along w i th itsRietve ldfit  pro f il e.  Th eg ood n es s o f  fi tting $\ ch i^ 2$ is  1.2 6 a n d th e l atti ce pa rameters of t heunit cel l are  a=5. 4549 (2 ) and  c=13. 3194( 2) . The oxygen co nten t is dete rmi ne d b ytherm o gravim etr icanalysi s which iscl o s e  t o its stoichiometr ic v al ue of 3. 0.

![ ( Co lo r  online)  X -ra y di f f racti on p a tt ern of L a$_{0. 7 5} $B a$_{0.2 5} $CoO$_ 3$  at  ro om te m pera ture.The soli d cir c les represents the experimen t al X -r a y di ffr action data , th e  red  lin e  o n t h e exp erime nt a ld ata exhibits the Ri et veld r efine ment for rhom bohedral R - 3 c  structu re w i th $\chi^2$=1.26,  theshort vert i cal line s sho w the Br agg peakp o sitions,  an d t hebot t o mblue line dis p l aysth e diffe ren ce betw een  th e e xpe ri mental an d calcul at ed  p at ter n.[]{ d ata-labe l= "fi g:  XR D"}]( F ig1.ep s){wi dth= "0 .6 \ col umnwidt h "} Resu lt sandDis cu ssion s
== = === ======= ========= =
T herm om ag netic i rreversibilit y---------- -- --- ------ - - -------
Figure \[fig: MT\] sho w s the m agn etiza tion  versus t emp eratur e c u rves a t thefield  o f 5 O e, 10 0 Oe , 5 00  Oe, and 1 0 0 00Oe in  f ield  cooled  (FC) and zero fie l d c ooled (ZFC) p rot ocol s .  I n F C  p r oto co l  th e sample is coole d to 5 K i np re sence of a p pli ed  fieldand dat a isr ecorded  in heati ng run wi th outc h ang ing the fi eld. InZFC proto c ol th e  s ample  is  coole dto5 K i n zero fie ld, t hen fi el d is a pplie d,  and dat a is recorded in the he atingrun.Bot h FC andZFC mag netizatio n cu rves exhib ita p arama gne t ic to  fer r om agn e tic t rans i tion on c o ol ing a nd  the transi t i o n t emper atu r e (T$_ C$)is estimated to b e  around 203 Kby t h e  te mpe r atur ederivative ofthe  5 0 0  Oe FC m ag netizationcurve (s ee inset  of Fi g. \[f ig: MT
. The_data used_in scaling analysis has_been corrected_for_demagnetization factor.

The_x-ray_data has been_analyzed by the_Rietveld refinement method using_FULLPROF software[@Carvajal] and_the_results show that the sample is single phase and crystallizes in rhombohedral structure with_space_group R-3c_which_is_in agrement with the previous_report.[@Fita] Figure \[fig: XRD\] displays the_room temperature_x-ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ along with its_Rietveld_fit profile. The_goodness of fitting $\chi^2$ is 1.26 and the lattice_parameters of the unit cell are_a=5.4549(2) and c=13.3194(2)._The_oxygen_content is determined by_thermogravimetric analysis which is close to_its stoichiometric value of 3.0.

![(Color online)_X-ray diffraction pattern of La$_{0.75}$Ba$_{0.25}$CoO$_3$ at room_temperature. The solid circles represents the_experimental X-ray diffraction data, the_red line_on the experimental data exhibits_the Rietveld refinement_for rhombohedral_R-3c structure with_$\chi^2$=1.26, the short vertical lines show_the Bragg peak_positions, and the bottom blue line_displays_the difference between_the_experimental_and calculated_pattern.[]{data-label="fig: XRD"}](Fig1.eps){width="0.6\columnwidth"}

Results and_Discussions
=======================

Thermomagnetic_irreversibility
------------------------------

Figure \[fig: MT\]_shows_the magnetization versus temperature curves at_the_field of 5 Oe, 100 Oe, 500 Oe, and 10000 Oe_in field cooled (FC)_and_zero field cooled (ZFC)_protocols. In FC protocol the_sample is cooled to 5 K in_presence of_applied field_and data is recorded in heating run without changing the field._In ZFC protocol the sample is_cooled to 5 K in_zero field,_then_field is applied,_and_data is_recorded in the heating run. Both FC_and ZFC_magnetization curves exhibit a paramagnetic to_ferromagnetic transition on cooling_and_the transition temperature (T$_C$) is estimated_to be around 203 K by the_temperature derivative of the 500 Oe_FC_magnetization_curve (see inset of Fig. \[fig:_MT